Phonons and Electron Correlations in HighTemperature and Other Novel Superconductors
View this Special IssueResearch Article  Open Access
R. A. Jishi, H. M. Alyahyaei, "Electronic and Lattice Dynamical Properties of the IronBased Superconductors LiFeAs and NaFeAs", Advances in Condensed Matter Physics, vol. 2010, Article ID 804343, 6 pages, 2010. https://doi.org/10.1155/2010/804343
Electronic and Lattice Dynamical Properties of the IronBased Superconductors LiFeAs and NaFeAs
Abstract
The electronic structure and lattice vibrational frequencies of the newly discovered superconductors, LiFeAs and NaFeAs, are calculated within density functional theory. We show that, in the vicinity of the Fermi energy, the density of states is dominated by contributions from Fe 3d states. We also calculate the electronphonon coupling strength and show that it is too weak to account for the observed values of the superconducting transition temperatures. This seems to indicate that the ironbased superconductors are not of the conventional type.
1. Introduction
A new class of layered, high superconductors has been recently discovered. Kamihara et al. [1] reported a superconducting transition temperature = 26 K in fluorinedoped LaFeAsO. Shortly afterwards, it was found that under pressure increased to 43 K [2]. Replacement of lanthanum with other rare earth metals gave a series of superconducting compounds , where Re = Ce, Pr, Nd, Sm, or Gd, with transition temperatures close to or exceeding 50 K [3–8]. Oxygen deficient samples were also synthesized and found to superconduct at 55 K [9–11]. Hole doping, through the partial substitution of La with Sr, or Gd with Th, was also found to yield superconducting compounds [12, 13]. Usinghigh pressure techniques, it was possible to increase the concentration of the Fdopant [14] and to synthesize superconducting compounds where La is replaced by the late rare earth elements Tb and Dy [15, 16]. The parent compound ReFeAsO is a layered compound consisting of a stack of alternating ReO and FeAs layers. Each ReO layer consists of an Osheet surrounded by two Re sheets. Similarly, each FeAs layer consists of an Fesheet surrounded by two As sheets such that each Fe atom is tetrahedrally coordinated to four As atoms. Neutron diffraction measurements [17–20] establish that the Fe magnetic moments adopt a collinear antiferromagnetic (cAFM) order whereby ferromagnetic chains are coupled antiferromagnetically along the direction orthogonal to the chains.
Superconductivity was also discovered in a second class of compounds containing FeAs layers, namely, , where A is an alkaline earth metal. Hole doping, by partial replacement of A with alkali metals, results in superconducting compounds with reaching 38 K in and [21–25]. Partial substitution of Fe with Co was also shown to give a superconducting compound with = 22 K [26]. Similarly to the first class, in the parent compounds the Fe magnetic moments in this second class have a collinear AFM order with a spinstripes pattern [27–29]. In both classes, the Fe magnetic moments in the parent compounds exhibit magnetic order, at low temperature, which disappears upon doping, making way for the emergence of superconductivity. This leads to the reasonable belief that strong electronic correlations are important in these systems, and that superconductivity in these compounds is somehow connected to magnetic fluctuations [30–42]. Indeed, the electronphonon coupling in LaOFeAs was estimated to be too small [43] to give rise to superconductivity within the conventional BCS formulation. [44]
Recently, a third class of ironbased superconductors was discovered. LiFeAs and NaFeAs were found to superconduct below 18 K and 9 K, respectively, [45–48]. It turns out that in these two compounds no magnetic order is detected at all temperatures. In some sense, these two compounds are important with regards to understanding the mechanism of superconductivity in ironbased superconductors. The absence of spin density wave (SDW) transition, on the one hand, and the relatively low in comparison with the first two classes of ironbased superconductors, on the other hand, make these two compounds possible candidates for being conventional BCS superconductors.
Band structure calculations, using local density approximation (LDA) within density functional theory (DFT), were recently reported for LiFeAs [49, 50]. It was found that LiFeAs is semimetallic, and that the density of states (DOSs) near the Fermi level is dominated by the Fe 3d states. Thus, the electronic structure of stoichiometric LiFeAs is similar to that of the parent compounds of the first class, with a hole cylinder at the Brillouin zone (BZ) center, electron cylinders at the BZ corners, and an electronic DOS that decreases strongly with increasing energy in the vicinity of the Fermi energy.
In this work we report DFT calculations of the electronic and lattice properties of LiFeAs and NaFeAs. In particular, we calculate the electronphonon coupling strength and show that it is too weak to account for the superconducting transition temperatures observed in these compounds. Our calculations, together with previous calculations [44] of the electronphonon coupling strength in LaOFeAs, seem to indicate that ironbased superconductors are not of the conventional type.
2. Method
The electronic structure calculations are carried out using the allelectron fullpotential linear augmented plane wave (FPLAPW) method as implemented in WIEN2K code [51]. The exchangecorrelation potential was calculated using the generalized gradient approximation (GGA) as proposed by Pedrew, Burke, and Ernzerhof (PBE) [52]. The radii of the muffintin spheres for the various atoms were chosen so that the neighboring spheres almost touch each other. We set the parameter , where is the smallest muffintin radius, and is a cutoff wave vector. The valence wave functions inside the muffintin spheres are expanded in terms of spherical harmonics up to , and in terms of plane waves with a wave vector cutoff in the interstitial region. The charge density is Fourier expanded up to , where is the Bohr radius. Convergence of the selfconsistent field calculations is attained with a total energy convergence tolerance of 0.01 mRy.
The calculation of the frequencies of the vibrational modes and the electronphonon coupling parameter was performed using ultrasoft pseudopotentials and an expansion of the wave function of the valence electrons in terms of plane waves, with an energy cutoff of 30 Rydbergs [53]. The charge density is Fourier expanded with an energy cutoff of 400 Rydbergs. The dynamical matrices and the electronphonon coupling parameter are calculated using DFT in the linear response approximation. In calculating the phonon frequencies, the electronic integration is carried out using a uniform mesh of points in the Brillouin zone. On the other hand, the electronic density of states, used in computing the electronphonon coupling parameter λ, is calculated using a finer mesh of points. The value of λ is obtained by averaging over a uniform mesh of phonon momentum points. The phonon dispersion curves are obtained by Fourier interpolation of the dynamical matrices computed on the points mesh.
In the electronic and lattice calculations, the experimental values of the lowtemperature lattice constants and atomic positions [45–48] are used. For both compounds, the crystal is tetragonal with space group P4/nmm. In LiFeAs, the lattice constants are = 3.76982 Å, = 6.30693 Å, whereas in NaFeAs, = 3.94729 Å, and = 6.99112 Å.
3. Results and Discussion
Our results for the electronic structure calculations for LiFeAs and NaFeAs are summarized in Figures 1 and 2, respectively, where the electronic density of states (DOSs) is displayed. For LiFeAs, our calculated DOS is similar to that reported earlier [49, 50]. In both LiFeAs and NaFeAs, the DOS plots show some generic features that are common to the parent compounds of the ironbased superconductors: a DOS that is dominated by the Fe 3d states in the vicinity of the Fermi energy, with only a small contribution from the As and alkali metal states and that is strongly decreasing with energy near the Fermi energy.
It should be noted that in a unit cell of LiFeAs, for example, there are two Li, two Fe, and two As atoms. Thus to get the total atomic DOS, the values of the atomic DOS shown in 1 should be multiplied by 2. The total DOS is the sum of the total atomic DOS and the DOS in the interstitial region.
Since the DOS at the Fermi energy, (), is ~4 states/eV in both LiFeAs and NaFeAs, which is not very small, and because of the relatively lower compared with the other ironbased superconductors, one may wonder whether electronphonon coupling may lie behind the mechanism for superconductivity in LiFeAs and NaFeAs. This notion may be given more credence by the observation that a sodium atom is about three times more massive than a lithium atom, so that if the attractive electronelectron interaction is mediated by the alkalimetal atomic vibrations, then this difference in the mass could explain the difference in the values of between the two compounds via the wellknown isotope effect.
To test this idea, we carried out a calculation of the phonon dispersion curves and the electronphonon coupling strength in these compounds. Since the crystallographic point group in LiFeAs and NaFeAs is , the vibrational modes at , the BZ center, are decomposed according to the following irreducible representations:
The acoustic modes, with vanishing frequency at , the BZ center, transform according to the and irreducible representations. Excluding the acoustic modes, we are left with 15 modes with nonzero frequencies; among these, the symmetric ones are Ramanactive, while the antisymmetric modes are infraredactive. The calculated frequencies of the Raman and infraredactive modes at the point of the BZ are given in Table 1. The phonon dispersion curves in LiFeAs, plotted along high symmetry directions in the BZ, are shown in Figure 3, and the corresponding curves in NaFeAs are given in Figure 4. Our results for the phonon frequencies at the BZ center may be checked by Raman scattering and infrared absorption experiments, while the phonon dispersion curves may be checked by neutron scattering measurements.

We calculated the electronphonon coupling parameter and found it to be 0.29 and 0.27 for LiFeAs and NaFeAs, respectively. For conventional superconductors, where the attractive electronelectron interaction is mediated by phonons, the transition temperature is given by the Allen and Dynes [54] modified McMillan's formula [55]
where is the logarithmic average phonon frequency, expressed in degrees Kelvin, and is the Coulomb pseudopotential parameter, usually taken to be ~0.13. Since in LiFeAs and NaFeAs is of the order of 100 K, the resulting value of is much less than 1 K. We conclude that the electronphonon coupling is too weak to account for superconductivity in this class of ironbased superconductors.
There are some puzzling questions that beset this third class of ironbased superconductors. In the parent compounds of the first two classes of ironbased superconductors, magnetic order is established at low temperatures, where the Fe magnetic moments adopt a collinear antiferromagnetic (cAFM) order with a stripelike pattern; this is unequivocally confirmed by both neutron diffraction measurements [17–20] and DFT calculations [31–39]. In the first class, it is only upon electron doping through the replacement of a small percentage of oxygen atoms with fluorine atoms, or the removal of a small percentage of oxygen atoms, that the magnetic order is suppressed and superconductivity emerges. In the second class of ironbased superconductors, magnetic order is suppressed by hole doping through the replacement of some alkaline earth atoms with alkali atoms. To better understand the situation in the third class of ironbased superconductors, we carried out spinpolarized DFT calculations on stoichiometric LiFeAs and NaFeAs, in addition to the calculations reported above for the nonmagnetic phases of these compounds. We considered, within GGA, various spin arrangements on the Fe sites. Similarly to the case of the first two classes, we find that the cAFM phase, with a spinstripes pattern, is indeed the lowest energy phase. Within GGA, the energy of the cAFM phase in LiFeAs is lower than the AFM phase by 0.081 eV per Fe atom (eV/Fe), lower than the ferromagnetic (FM) phase by 0.085 eV/Fe, and lower than the nonmagnetic phase by 0.123 eV/Fe. For NaFeAs, the energy of the cAFM phase is lower than the AFM phase by 0.048 eV/Fe, lower than the FM phase by 0.205 eV/Fe, and lower than the nonmagnetic phase by 0.182 eV/Fe. The calculated magnetic moment on an Fe site is 2.18 in the case of NaFeAs, and 1.76 in the case of LiFeAs, where is the Bohr magneton. Thus, according to our DFT calculations, stoichiometric LiFeAs and NaFeAs should be similar to the parent compounds of the first two classes, and they should not superconduct; instead, at low temperature, the stoichiometric compounds should display magnetic order. Deviations from stoichiometry, on the other hand, may suppress the magnetic order, making way for superconductivity, just like doping does in the first two classes of ironbased compounds. In the case of LiFeAs, it is indeed the case that the synthesized superconducting compounds were not stoichiometric, the chemical formula being FeAs [47]. The situation is less clear in the case of NaFeAs [48], but we believe, on the basis of our spinpolarized calculations and the absence of any detectable magnetic order at low temperatures, that the synthesized NaFeAs samples may also be nonstoichiometric.
We should note, however, that our results on the magnetic structure of the third class of compounds are only tentative. One problem is that the calculated magnetic moment per Fe site is too large in comparison with the experimental value in LaFeAsO, where the Fe moments also adopt cAFM order, albeit with a magnetic moment of only 0.36 [17]. It has been shown by various groups [56–58] that even though the Fe moments adopt the stripeAFM order in the undoped LaFeAsO compound, yet the stabilization energy and the value of the Fe magnetic moment are sensitive to the type of exchangecorrelation functional employed in the calculation, and to the position of the As atom. At this point, all we can say is that DFT calculations within GGA using PBE exchange correlation potential suggest that stoichiometric LiFeAs and NaFeAs compounds will display magnetic order at low temperatures.
4. Conclusions
In conclusion, we have presented the results of electronic structure calculations on LiFeAs and NaFeAs, members of a new class of superconducting compounds. In similarity to other ironbased superconductors, the density of states in the vicinity of the Fermi energy is found to be dominated by contributions from the Fe 3d states. We have also calculated the Raman and infrared phonon frequencies at the Brillouin zone center, as well the phonon dispersion curves along high symmetry directions in the Brillouin zone. We have evaluated the electronphonon coupling parameter in LiFeAs and NaFeAs and found its value to be too small to account for the observed superconducting transition temperatures in these compounds. Our results, taken together with previous estimates of the electronphonon coupling strength in LaFeAsO, seem to suggest clearly that ironbased superconductors are not of the conventional type, where the attractive electronelectron interaction is mediated by phonons.
References
 Y. Kamihara, T. Watanabe, M. Hirano, and H. Hosono, “Ironbased layered superconductor La[${\text{O}}_{1x}{\text{F}}_{x}$]FeAs ($x=0.05$0.12) with $\text{Tc}=26$ K,” Journal of the American Chemical Society, vol. 130, no. 11, pp. 3296–3297, 2008. View at: Publisher Site  Google Scholar
 H. Takahashi, K. Igawa, K. Arii, Y. Kamihara, M. Hirano, and H. Hosono, “Superconductivity at 43 K in an ironbased layered compound ${\text{LaO}}_{1x}{\text{F}}_{x}$FeAs,” Nature, vol. 453, no. 7193, pp. 376–378, 2008. View at: Publisher Site  Google Scholar
 G. F. Chen, Z. Li, D. Wu et al., “Superconductivity at 41 K and its competition with spindensitywave instability in layered Ce${\text{O}}_{1x}{\text{F}}_{x}$FeAs,” Physical Review Letters, vol. 100, no. 24, Article ID 247002, 2008. View at: Publisher Site  Google Scholar
 Z.A. Ren, J. Yang, W. Lu et al., “Superconductivity at 52 K in iron based F doped layered quaternary compound Pr[${\text{O}}_{1x}{\text{F}}_{x}$] FeAs,” Materials Research Innovations, vol. 12, no. 3, pp. 105–106, 2008. View at: Publisher Site  Google Scholar
 Z.A. Ren, J. Yang, W. Lu et al., “Superconductivity in the ironbased Fdoped layered quaternary compound Nd[${\text{O}}_{1x}{\text{F}}_{x}$]FeAs,” Europhysics Letters, vol. 82, no. 5, Article ID 57002, 2008. View at: Publisher Site  Google Scholar
 X. H. Chen, T. Wu, G. Wu, R. H. Liu, H. Chen, and D. F. Fang, “Superconductivity at 43 K in SmFeAs${\text{O}}_{1x}{\text{F}}_{x}$,” Nature, vol. 453, no. 7196, pp. 761–762, 2008. View at: Publisher Site  Google Scholar
 Z.A. Ren, W. Lu, J. Yang et al., “Superconductivity at 55 K in ironbased Fdoped layered quaternary compound Sm[${\text{O}}_{1x}{\text{F}}_{x}$] FeAs,” Chinese Physics Letters, vol. 25, no. 6, pp. 2215–2216, 2008. View at: Publisher Site  Google Scholar
 P. Cheng, L. Fang, H. Yang et al., “Superconductivity at 36 K in gadoliniumarsenide oxides Gd${\text{O}}_{1x}{\text{F}}_{x}$FeAs,” Science in China, Series G, vol. 51, no. 6, pp. 719–722, 2008. View at: Publisher Site  Google Scholar
 J. Yang, Z.C. Li, W. Lu et al., “Superconductivity at 53.5 K in GdFeAsO1$d$,” Superconductor Science and Technology, vol. 21, no. 8, Article ID 082001, 2008. View at: Publisher Site  Google Scholar
 G. Wu, Y. J. Yan, T. Wu et al., “Superconductivity induced by oxygen deficiency in La0.85 Sr0.15 FeAsO1$d$,” Physical Review B, vol. 78, no. 9, Article ID 092503, 2008. View at: Publisher Site  Google Scholar
 Z.A. Ren, G.C. Che, X.L. Dong et al., “Superconductivity and phase diagram in ironbased arsenicoxides ReFeAsO1$d$ ($\text{Re}=\text{rare}$earth metal) without fluorine doping,” Europhysics Letters, vol. 83, no. 1, Article ID 17002, 2008. View at: Publisher Site  Google Scholar
 H.H. Wen, G. Mu, L. Fang, H. Yang, and X. Zhu, “Superconductivity at 25 K in holedoped (${\text{La}}_{1x}{\text{Sr}}_{x}$)OFeAs,” Europhysics Letters, vol. 82, no. 1, Article ID 17009, 2008. View at: Publisher Site  Google Scholar
 C. Wang, L. Li, S. Chi et al., “Thoriumdopinginduced superconductivity up to 56 K in ${\text{Gd}}_{1x}{\text{Th}}_{x}$FeAsO,” Europhysics Letters, vol. 83, no. 6, Article ID 67006, 2008. View at: Publisher Site  Google Scholar
 W. Lu, X.L. Shen, J. Yang et al., “Superconductivity at 41.0 K in the Fdoped LaFeAs${\text{O}}_{1x}{\text{F}}_{x}$,” Solid State Communications, vol. 148, no. 34, pp. 168–170, 2008. View at: Publisher Site  Google Scholar
 J.W. G. Bos, G. B. S. Penny, J. A. Rodgers, D. A. Sokolov, A. D. Huxley, and J. P. Attfield, “High pressure synthesis of late rare earth RFeAs(O,F) superconductors; $\text{R}=\text{Tb}$ and Dy,” Chemical Communications, no. 31, pp. 3634–3635, 2008. View at: Publisher Site  Google Scholar
 L.J. Li, Y.K. Li, Z.A. Ren et al., “Superconductivity above 50 K in ${\text{Tb}}_{1x}{\text{Th}}_{x}$FeAsO,” Physical Review B, vol. 78, no. 13, Article ID 132506, 2008. View at: Publisher Site  Google Scholar
 C. de la Cruz, Q. Huang, J. W. Lynn et al., “Magnetic order close to superconductivity in the ironbased layered La${\text{O}}_{1x}{\text{F}}_{x}$FeAs systems,” Nature, vol. 453, no. 7197, pp. 899–902, 2008. View at: Publisher Site  Google Scholar
 J. Zhao, Q. Huang, C. de la Cruz et al., “Structural and magnetic phase diagram of CeFeAs${\text{O}}_{1x}{\text{F}}_{x}$ and its relation to hightemperature superconductivity,” Nature Materials, vol. 7, no. 12, pp. 953–959, 2008. View at: Publisher Site  Google Scholar
 J. Zhao, Q. Huang, C. de la Cruz et al., “Lattice and magnetic structures of PrFeAsO, PrFeAsO0.85F 0.15, and PrFeAsO0.85,” Physical Review B, vol. 78, no. 13, Article ID 132504, 2008. View at: Publisher Site  Google Scholar
 Y. Qiu, W. Bao, Q. Huang et al., “Crystal structure and antiferromagnetic order in NdFeAs${\text{O}}_{1x}{\text{F}}_{x}$ ($x=0.0$ and 0.2) superconducting compounds from neutron diffraction measurements,” Physical Review Letters, vol. 101, no. 25, Article ID 257002, 2008. View at: Publisher Site  Google Scholar
 M. Rotter, M. Tegel, and D. Johrendt, “Superconductivity at 38 K in the iron arsenide (${\text{Ba}}_{1x}{\text{K}}_{x}$)${\text{Fe}}_{2}{\text{As}}_{2}$,” Physical Review Letters, vol. 101, no. 10, Article ID 107006, 2008. View at: Publisher Site  Google Scholar
 G.F. Chen, Z. Li, G. Li et al., “Superconductivity in holedoped (${\text{Sr}}_{1x}{\text{K}}_{x}$)${\text{Fe}}_{2}{\text{As}}_{2}$,” Chinese Physics Letters, vol. 25, no. 9, pp. 3403–3405, 2008. View at: Publisher Site  Google Scholar
 K. Sasmal, B. Lv, B. Lorenz et al., “Superconducting febased compounds (${\text{A}}_{1x}{\text{Sr}}_{x}$)${\text{Fe}}_{2}{\text{As}}_{2}$ with $\text{A}=\text{K}$ and Cs with transition temperatures up to 37 K,” Physical Review Letters, vol. 101, no. 10, Article ID 107007, 2008. View at: Publisher Site  Google Scholar
 G. Wu, R. H. Liu, Y. J. Yan et al., “Transport properties and superconductivity in Ba1xM x${\text{Fe}}_{2}{\text{As}}_{2}$ ($\text{M}=\text{La}$ and K) with double FeAs layers,” Europhysics Letters, vol. 84, no. 2, Article ID 27010, 2008. View at: Publisher Site  Google Scholar
 N. Ni, S. L. Bud'ko, A. Kreyssig et al., “Anisotropic thermodynamic and transport properties of singlecrystalline ${\text{Ba}}_{1x}{\text{K}}_{x}$${\text{Fe}}_{2}{\text{As}}_{2}$ ($x=0$ and 0.45),” Physical Review B, vol. 78, no. 1, Article ID 014507, 2008. View at: Publisher Site  Google Scholar
 A. S. Sefat, R. Jin, M. A. McGuire, B. C. Sales, D. J. Singh, and D. Mandrus, “Superconductivity at 22 K in codoped Ba${\text{Fe}}_{2}{\text{As}}_{2}$ crystals,” Physical Review Letters, vol. 101, no. 11, Article ID 117004, 2008. View at: Publisher Site  Google Scholar
 Q. Huang, Y. Qiu, W. Bao et al., “Neutrondiffraction measurements of magnetic order and a structural transition in the parent Ba${\text{Fe}}_{2}{\text{As}}_{2}$ compound of FeAsbased hightemperature superconductors,” Physical Review Letters, vol. 101, no. 25, Article ID 257003, 2008. View at: Publisher Site  Google Scholar
 K. Kitagawa, N. Katayama, K. Ohgushi, M. Yoshida, and M. Takigawa, “Commensurate itinerant antiferromagnetism in ${\text{BaFe}}_{2}{\text{As}}_{2}$: 75AsNMR studies on a selfflux grown single crystal,” Journal of the Physical Society of Japan, vol. 77, no. 11, Article ID 114709, 2008. View at: Publisher Site  Google Scholar
 Y. Su, P. Link, A. Schneidewind et al., “Antiferromagnetic ordering and structural phase transition in ${\text{Ba}}_{2}{\text{Fe}}_{2}{\text{As}}_{2}$ with Sn incorporated from the growth flux,” Physical Review B, vol. 79, no. 6, Article ID 064504, 2009. View at: Publisher Site  Google Scholar
 D. J. Singh and M.H. Du, “Density functional study of LaFeAs${\text{O}}_{1x}{\text{F}}_{x}$: a low carrier density superconductor near itinerant magnetism,” Physical Review Letters, vol. 100, no. 23, Article ID 237003, 2008. View at: Publisher Site  Google Scholar
 K. Haule, J. H. Shim, and G. Kotliar, “Correlated electronic structure of La${\text{O}}_{1x}{\text{F}}_{x}$FeAs,” Physical Review Letters, vol. 100, no. 22, Article ID 226402, 2008. View at: Publisher Site  Google Scholar
 J. Dong, H. J. Zhang, G. Xu et al., “Competing orders and spindensitywave instability in La(${\text{O}}_{1x}{\text{F}}_{x}$)FeAs,” Europhysics Letters, vol. 83, no. 2, Article ID 27006, 2008. View at: Publisher Site  Google Scholar
 F. Ma and Z.Y. Lu, “Ironbased layered compound LaFeAsO is an antiferromagnetic semimetal,” Physical Review B, vol. 78, no. 3, Article ID 033111, 2008. View at: Publisher Site  Google Scholar
 C. Cao, P. J. Hirschfeld, and H.P. Cheng, “Proximity of antiferromagnetism and superconductivity in LaFeAs${\text{O}}_{1x}{\text{F}}_{x}$: effective Hamiltonian from ab initio studies,” Physical Review B, vol. 77, no. 22, Article ID 220506, 2008. View at: Publisher Site  Google Scholar
 T. Yildirim, “Origin of the 150K anomaly in LaFeAsO: competing antiferromagnetic interactions, frustration, and a structural phase transition,” Physical Review Letters, vol. 101, no. 5, Article ID 057010, 2008. View at: Publisher Site  Google Scholar
 Z. Y. Weng, “Hidden SDW order and effective lowenergy theory for FeAs superconductors,” Physica E: Lowdimensional Systems and Nanostructures, vol. 41, no. 7, pp. 1281–1284, 2009. View at: Google Scholar
 F. Ma, Z.Y. Lu, and T. Xiang, “Arsenicbridged antiferromagnetic superexchange interactions in LaFeAsO,” Physical Review B, vol. 78, no. 22, Article ID 224517, 2008. View at: Publisher Site  Google Scholar
 Z. P. Yin, S. Lebègue, M. J. Han, B. P. Neal, S. Y. Savrasov, and W. E. Pickett, “Electronhole symmetry and magnetic coupling in antiferromagnetic LaFeAsO,” Physical Review Letters, vol. 101, no. 4, Article ID 047001, 2008. View at: Publisher Site  Google Scholar
 S. Ishibashi, K. Terakura, and H. Hosono, “A possible ground state and its electronic structure of a mother material (LaOFeAs) of new superconductors,” Journal of the Physical Society of Japan, vol. 77, no. 5, Article ID 053709, 2008. View at: Publisher Site  Google Scholar
 Q. Si and E. Abrahams, “Strong correlations and magnetic frustration in the high Tc iron pnictides,” Physical Review Letters, vol. 101, no. 7, Article ID 076401, 2008. View at: Publisher Site  Google Scholar
 C. Fang, H. Yao, W.F. Tsai, J. Hu, and S. A. Kivelson, “Theory of electron nematic order in LaFeAsO,” Physical Review B, vol. 77, no. 22, Article ID 224509, 2008. View at: Publisher Site  Google Scholar
 C. Xu, M. Müller, and S. Sachdev, “Ising and spin orders in the ironbased superconductors,” Physical Review B, vol. 78, no. 2, Article ID 020501, 2008. View at: Publisher Site  Google Scholar
 L. Boeri, O. V. Dolgov, and A. A. Golubov, “Is LaFeAs${\text{O}}_{1x}{\text{F}}_{x}$ an electronphonon superconductor?” Physical Review Letters, vol. 101, no. 2, Article ID 026403, 2008. View at: Publisher Site  Google Scholar
 J. Bardeen, L. N. Cooper, and J. R. Schrieffer, “Theory of superconductivity,” Physical Review, vol. 108, no. 5, pp. 1175–1204, 1957. View at: Publisher Site  Google Scholar
 M. J. Pitcher, D. R. Parker, P. Adamson et al., “Structure and superconductivity of LiFeAs,” Chemical Communications, no. 45, pp. 5918–5920, 2008. View at: Publisher Site  Google Scholar
 J. H. Tapp, Z. Tang, B. Lv et al., “LiFeAs: an intrinsic FeAsbased superconductor with $\text{Tc}=18$ K,” Physical Review B, vol. 78, no. 6, Article ID 060505, 2008. View at: Publisher Site  Google Scholar
 X. C. Wang, Q. Q. Liu, Y. X. Lv et al., “The superconductivity at 18 K in LiFeAs system,” Solid State Communications, vol. 148, no. 1112, pp. 538–540, 2008. View at: Publisher Site  Google Scholar
 D. R. Parker, M. J. Pitcher, P. J Baker et al., “Structure, antiferromagnetism and superconductivity of the layered iron arsenide NaFeAs,” Chemical Communications Articles, pp. 2189–2191, 2009. View at: Google Scholar
 I. A. Nekrasov, Z. V. Pchelkina, and M. V. Sadovskii, “Electronic structure of new LiFeAs highTc superconductor,” JETP Letters, vol. 88, no. 8, pp. 543–545, 2008. View at: Publisher Site  Google Scholar
 D. J. Singh, “Electronic structure and doping in ${\text{BaFe}}_{2}{\text{As}}_{2}$ and LiFeAs: density functional calculations,” Physical Review B, vol. 78, no. 9, Article ID 094511, 2008. View at: Publisher Site  Google Scholar
 P. Blaha, K. Schwarz, G. K. H. Madsen, D. Kavasnicka, and J. Luitz, WIEN2K, An Augmented Plane Wave + Local Orbitals Program for Calculating Crystal Properties, Technische Universität, Wien, Austria, 2001.
 J. P. Perdew, K. Burke, and M. Ernzerhof, “Generalized gradient approximation made simple,” Physical Review Letters, vol. 77, no. 18, pp. 3865–3868, 1996. View at: Google Scholar
 P. Giannozzi et al., http://www.quantumespresso.org.
 P. B. Allen and R. C. Dynes, “Transition temperature of strongcoupled superconductors reanalyzed,” Physical Review B, vol. 12, no. 3, pp. 905–922, 1975. View at: Publisher Site  Google Scholar
 W. L. McMillan, “Transition temperature of strongcoupled superconductors,” Physical Review, vol. 167, no. 2, pp. 331–344, 1968. View at: Publisher Site  Google Scholar
 I. I. Mazin, M. D. Johannes, L. Boeri, K. Koepernik, and D. J. Singh, “Problems with reconciling density functional theory calculations with experiment in ferropnictides,” Physical Review B, vol. 78, no. 8, Article ID 085104, 2008. View at: Publisher Site  Google Scholar
 A. N. Yaresko, G.Q. Liu, V. N. Antonov, and O. K. Andersen, “Interplay between magnetic properties and Fermi surface nesting in iron pnictides,” Physical Review B, vol. 79, no. 14, Article ID 144421, 2009. View at: Publisher Site  Google Scholar
 S. Sharma, J. K. Dewhurst, S. Shallcross et al., “Magnetic properties of La${\text{O}}_{1x}{\text{F}}_{x}$FeAs,” http://arxiv.org/abs/0810.4278. View at: Google Scholar
Copyright
Copyright © 2010 R. A. Jishi and H. M. Alyahyaei. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.